Mahdi Nejatianfar | Batool Akhlaghinia | Roya Jahanshahiprofdoc.um.ac.ir/articles/a/1064938.pdf ·...
Embed Size (px)
Transcript of Mahdi Nejatianfar | Batool Akhlaghinia | Roya Jahanshahiprofdoc.um.ac.ir/articles/a/1064938.pdf ·...
Received: 4 May 2017 Revised: 14 August 2017 Accepted: 15 August 2017
FU L L PAP ER
Cu(II) immobilized on guanidinated epibromohydrin‐functionalized γ‐[email protected] (γ‐[email protected]‐EG‐Cu(II)):A highly efficient magnetically separable heterogeneousnanocatalyst for one‐pot synthesis of highly substitutedimidazoles
Mahdi Nejatianfar | Batool Akhlaghinia | Roya Jahanshahi
Department of Chemistry, Faculty ofSciences, Ferdowsi University of Mashhad,Mashhad 9177948974, Iran
CorrespondenceBatool Akhlaghinia, Department ofChemistry, Faculty of Sciences, FerdowsiUniversity of Mashhad, Mashhad9177948974, Iran.Email: [email protected]
Appl Organometal Chem. 2017;e4095.https://doi.org/10.1002/aoc.4095
A simple, efficient and eco‐friendly procedure has been developed using Cu(II)
immobilized on guanidinated epibromohydrin‐functionalized γ‐[email protected]
(γ‐[email protected]‐EG‐Cu(II)) for the synthesis of 2,4,5‐trisubstituted and 1,2,4,5‐
tetrasubstituted imidazoles, via the condensation reactions of various aldehydes
with benzil and ammoniumacetate or ammoniumacetate and amines, under sol-
vent‐free conditions. High‐resolution transmission electron microscopy analysis
of this catalyst clearly affirmed the formation of a γ‐Fe2O3 core and a TiO2 shell,
with mean sizes of about 10–20 and 5–10 nm, respectively. These data were in
very good agreement with X‐ray crystallographic measurements (13 and 7 nm).
Moreover, magnetization measurements revealed that both γ‐[email protected] and
γ‐Fe2O[email protected]‐EG‐Cu(II) had superparamagnetic behaviour with saturation
magnetization of 23.79 and 22.12 emu g−1, respectively. γ‐[email protected]‐EG‐
Cu(II) was found to be a green and highly efficient nanocatalyst, which could
be easily handled, recovered and reused several times without significant loss of
its activity. The scope of the presented methodology is quite broad; a variety of
aldehydes as well as amines have been shown to be viable substrates. A mecha-
nism for the cyclocondensation reaction has also been proposed.
Cu(II) immobilized on guanidinated epibromohydrin‐functionalized γ‐[email protected] (γ‐[email protected]‐
EG‐Cu(II)), heterogeneous nanocatalyst, solvent‐free, substituted imidazoles
1 | INTRODUCTION
Imidazole ring‐containing compounds, which are a subsetof nitrogen‐containing heterocyclic compounds, exhibitwide ranges of biological and pharmacological activitiesthat make them very attractive compounds for organicchemists.[1,2] Many substituted imidazoles are known asbiocides (in particular, herbicides, fungicides andgrowth 2regulators), potent angiotensin II receptor
antagonists, glucagon receptor antagonists and inhib-itors of interleukin‐1 and 5‐lipoxygenase. Using imidaz-oles in ionic liquids and in N‐heterocyclic carbenes
has given a new dimension to the area of organometallicsand ‘green chemistry’. Also, imidazole derivatives havebeen used in photography as photosensitive compounds
and also as useful building blocks for the synthesis ofother classes of compounds. Therefore, the developmentof novel synthetic methods towards the preparation of
Copyright © 2017 John Wiley & Sons, Ltd.al/aoc 1 of 12
2 of 12 NEJATIANFAR ET AL.
substituted imidazoles has become an important target inrecent years.
The traditional approaches for the preparation of both2,4,5‐trisubstituted and 1,2,4,5‐tetrasubstituted imidazolesare mainly based on the cyclocondensation reaction of a1,2‐diketone with an aldehyde and a nitrogen source(ammonium acetate or ammonium acetate and amine).
Literature survey reveals that a great variety of catalysts,promoters and solvents have been developed for the syn-thesis of both 2,4,5‐trisubstituted and 1,2,4,5‐tetrasubstituted imidazoles, including the use of n‐PeFBA, HClO4–SiO2,
 zeolite HY, WD/SiO2,
RFOH/SBA‐15‐Pr‐SO3H, SZ, Fe3O4, Fe3O4–
PEG–Cu, InCl3⋅3H2O, NiCl2⋅6H2O,
K5CoW12O40⋅3H2O, silica gel/NaHSO4,
 moleculariodine, heteropolyacids, MW/Al2O3,
 trichloroisocyanuric acid, benzotriazole, ZrCl4,
 aceticacid, silica‐supported sulfuric acid, CAN,
 GO–chitosan, DABCO,
FeCl3⋅6H2O, mercaptopropylsilica, L‐proline,
MCM‐41 or p‐TsOH, and 1‐butyl‐3‐methylimidazoliumbromide. Despite the many methods available forthe synthesis of 2,4,5‐trisubstituted and 1,2,4,5‐tetrasubstituted imidazoles, most of these procedures suf-fer from one or more serious drawbacks such as use ofexpensive and hazardous acid catalysts, using toxic metalcatalysts, harsh reaction conditions, occurrence of sidereactions, laborious and complex work‐up and purifica-tion, high temperature, long reaction time, low yields andusing expensive and excess reagents. Therefore, the devel-opment of a new, green, high‐yielding, mild and efficientcatalytic system to overcome these shortcomings alongwith introducing a mild, efficient and environmentallybenign protocol for the synthesis of highly substitutedimidazoles is an important task in the planning ofsubstituted imidazole synthesis.
In continuation of our efforts to explore the catalyticactivity of heterogeneous Lewis and Brønsted acids forvarious organic transformations, we report hereina simple, mild and expeditious synthesis of 2,4,5‐trisubsti-tuted and 1,2,4,5‐tetrasubstituted imidazoles in highyields, using Cu(II) immobilized on guanidinatedepibromohydrin‐functionalized γ‐[email protected] (γ‐[email protected]‐EG‐Cu(II)) as an effectual catalyst.
2 | EXPERIMENTAL
2.1 | General
All chemical reagents and solvents were purchasedfrom Merck and Sigma‐Aldrich and were used asreceived without further purification. The purity
determinations of the products and the progress ofthe reactions were accomplished by TLC on silica gelpolygram STL G/UV 254 plates. Melting points of theproducts were determined with an Electrothermal Type9100 melting point apparatus. Fourier transform infra-red (FT‐IR) spectra were recorded with pressed KBrpellets using an AVATAR 370 FT‐IR spectrometer(Thermo Nicolet, USA) at room temperature in therange 400–4000 cm−1, with a resolution of 4 cm−1,and each spectrum was the average of 32 scans. NMRspectra were obtained with a Bruker Avance NMRspectrometer at 300 MHz, using CDCl3 and DMSO‐d6solvents in the presence of tetramethylsilane as theinternal standard. Elemental analyses were performedusing a Thermo Finnigan Flash EA 1112 Series instru-ment (furnace: 900 °C; oven: 65 °C; flow carrier:140 ml min−1; flow reference: 100 ml min−1). Massspectra were recorded with a CH7A VarianmatBremem instrument at 70 eV with electron impactionization. Thermogravimetric analysis (TGA) and dif-ferential thermogravimetry (DTG) were carried outusing a Shimadzu TG‐50 thermogravimetric analyserin the temperature range 25–900 °C at a heating rateof 10 °C min−1, under air atmosphere. High‐resolutiontransmission electron microscopy (HRTEM) was per-formed using a Philips CM30 microscope. Inductivelycoupled plasma (ICP) analysis was conducted with aVISTA‐PRO, CCD (Varian, Australia). Elemental com-positions were determined using energy‐dispersive spec-troscopy (EDS; SC7620) with a 133 eV resolution at20 kV. Room temperature magnetization isothermswere obtained using vibrating sample magnetometry(VSM; LakeShore 7400). Powder X‐ray diffraction(XRD) was performed using an X'Pert Pro MPD diffrac-tometer with Cu Kα (λ = 0.154 nm) radiation. Allyields refer to isolated products after purification byrecrystallization. γ‐[email protected]‐EG‐Cu(II) nanoparticleswere prepared using a method previously reported inthe literature.[41a]
2.2 | Typical procedure for preparation of2,4,5‐Triphenyl‐1H‐imidazole (3a)
γ‐[email protected]‐EG‐Cu(II) nanoparticles (2.5 mol%,0.030 g) were added to a mixture of benzil (1 mmol,0.210 g), benzaldehyde (1 mmol, 0.106 g) and NH4OAc(2.5 mmol, 0.192 g). The resulting mixture was stirredat 100 °C under neat conditions, until the reaction wasjudged to be complete by TLC (eluent = n‐hexane–ethylacetate, 7:3). After cooling to room temperature, hotethanol (5 ml) was added to the reaction mixture andthe catalyst was separated from the solution using an
NEJATIANFAR ET AL. 3 of 12
external magnet, washed with ethanol (2 × 10 ml) andair‐dried to be ready for the next run. Thereafter, theresultant mixture was concentrated under rotaryvacuum evaporation and the obtained crude productwas recrystallized from ethanol to afford the pure2,4,5‐triphenyl‐1H‐imidazole (0.290 g, 98%).
2.3 | Typical procedure for preparation of1,2,4,5‐Tetraphenylimidazole (3 t)
γ‐[email protected]‐EG‐Cu(II) nanoparticles (2.5 mol%,0.030 g,) were added to a mixture of benzil (1 mmol,0.210 g), benzaldehyde (1 mmol, 0.106 g), NH4OAc(1.5 mmol, 0.115 g) and aniline (1 mmol, 0.093 g). Theresulting mixture was stirred at 100 °C under neatconditions, until the reaction was judged to be completeby TLC (eluent = n‐hexane–ethyl acetate, 7:3). Aftercooling to room temperature, hot ethanol (5 ml) wasadded to the reaction mixture and the catalyst wasseparated from the solution using an external magnet,washed with ethanol (2 × 10 ml) and air‐dried to be readyfor the next run. Afterwards, the resultant mixture wasconcentrated under rotary vacuum evaporation and the
SCHEME 1 Overview of γ‐[email protected]‐EG‐Cu(II) preparation
obtained crude product was recrystallized from ethanolto afford pure 1,2,4,5‐tetraphenylimidazole (0.364 g, 98%).
3 | RESULTS AND DISCUSSION
Nanomagnetic catalysts have received a great deal ofattention in organic chemistry due to their easyseparation from reaction mixtures using an externalmagnet (which is not time‐consuming in comparisonwith the standard methods), clean forward reactions,and their having remarkable physical and chemicalproperties by controlling particle size and surface area.Recently, we successfully synthesized γ‐[email protected]‐
EG‐Cu(II) as a novel and magnetically recyclableheterogeneous nanocatalyst[41a] (Scheme 1). The cata-lytic activity of the synthesized nanocatalyst wasinitially investigated in the one‐pot synthesis of 1,4‐disubstituted 1,2,3‐triazoles, through alkyne–azidecycloaddition reactions, in water.[41a]
In the present study we decided to extend theapplication of γ‐[email protected]‐EG‐Cu(II) as a reusablesolid acid nanomagnetic catalyst towards the efficientsynthesis of 2,4,5‐trisubstituted and 1,2,4,5‐
SCHEME 2 Synthesis of 2,4,5‐
trisubstituted and 1,2,4,5‐tetrasubstituted
imidazoles via one‐pot condensation
reactions of aldehydes with benzil and
ammonium acetate or ammonium acetate
and amines in the presence of γ‐[email protected]‐EG‐Cu(II)
4 of 12 NEJATIANFAR ET AL.
tetrasubstituted imidazoles via one‐pot condensationreactions of aldehydes with benzil and ammoniumacetate or ammonium acetate and amines (Scheme 2).
FIGURE 2 XRD pattern of γ‐[email protected]
FIGURE 1 FT‐IR spectra of (a) γ‐[email protected] nanoparticles,
(b) epibromohydrin‐functionalized γ‐[email protected]‐E, (c) guanidinated
epibromohydrin‐functionalized γ‐[email protected]‐EG, (d) γ‐[email protected]‐
EG‐Cu(II)) and (e) γ‐[email protected]‐EG‐Cu(II) recovered after sixth run
3.1 | Characterization of γ‐[email protected]‐
The γ‐[email protected]‐EG‐Cu(II) catalyst synthesizedbased on the pathway described in Scheme 1 was thenfully characterized using various techniques includingFT‐IR spectroscopy, powder XRD, HRTEM, TGA/DTG, EDS, VSM, ICP analysis and elemental analysis(CHNS).
FT‐IR spectroscopy was engaged to compare thesynthesized γ‐[email protected], epibromohydrin‐functional-ized γ‐[email protected], guanidinated epibromohydrin‐func-tionalized γ‐[email protected] and γ‐[email protected]‐EG‐Cu(II)(Figure 1). The characteristic absorption band related tothe stretching vibration of Fe─O bond in γ‐Fe2O3 waspresent at about 571–698 cm−1, which was covered bythe broad absorption band of Ti─O in the TiO2 latticeat 500–850 cm−1. Also, the absorption band at1619 cm−1 and the broad band appearing at3100–3500 cm−1 were in turn associated with bendingand stretching vibrations of the adsorbed water moleculesand the surface‐attached hydroxyl groups (Figure 1a).
Immobilization of the epoxy ring to γ‐[email protected] frame-work was identified by the methylene C─H stretchingand bending vibration bands appearing at around2872–2923 and 1454 cm−1, respectively (Figure 1b).
Moreover, C─O─C vibrational stretching modes werevisualized at 1112 cm−1. These findings indicated thesuccessful grafting of epoxy rings to the γ‐[email protected]
surface. Evidence for the ring opening of epoxy with gua-nidine groups was the appearance of indicative bands ataround 3378 and 1454 cm−1, which were related toN─H and C─N stretching vibrations, respectively(Figure 1c).[44c] After coordination with Cu(II), the
diagnostic absorption bands corresponding to Cu─N andCu─O vibrations were observed at 428 and 450 cm−1,respectively.[41b] The respective bands were covered bystretching vibration modes of Fe─O and Ti─O bonds.Furthermore, ─NH2 and probably ─OH stretching
NEJATIANFAR ET AL. 5 of 12
frequencies (at around 3162–3378 cm−1) were shifted tolower wavenumber as a result of the metallation process.In addition, NH and probably OH bending vibrations(positioned at 1617 and 1619 cm−1, respectively) were alsoshifted to lower frequencies after coordination withCu(II). Likewise, C─N and C═N stretching vibrations(positioned at 1454 and 1662 cm−1) were shifted to lowerwavenumbers due to the metallation process (Figure 1d).On the other hand, bands at 1634 and 1401 cm−1 in thespectrum of γ‐[email protected]‐EG‐Cu(II) were related toCOO (in acetate), which proved the presence of Cu inthe catalyst. The mentioned absorption bands were cov-ered by broad stretching vibration frequencies related toC─N bond. Accordingly, potent metal–ligand interactionwas confirmed.
Powder XRD measurement was accomplished toidentify the crystalline structure of γ‐[email protected] shown in Figure 2, the reflection planes of (2 2 0),(3 1 1), (4 0 0), (4 2 2), (5 1 1) and (4 4 0), which areascribed to the cubic structure of γ‐Fe2O3 (JCPDS file
FIGURE 3 HRTEM images of γ‐[email protected]‐EG‐Cu(II)
FIGURE 4 TGA/DTG thermograms of
no. 04–0755), were readily recognized from the XRD pat-tern. Moreover, the existence of weak diffraction peaksrelating to (0 1 1), (0 0 4) and (0 2 0) crystallographic facescould be assigned to anatase XRD diffraction peaks.Accordingly, the average crystallite sizes of γ‐Fe2O3
and TiO2 (anatase) which were calculated using theDebye–Scherrer equation were approximately 13 and7 nm, respectively.
According to the HRTEM images of the catalyst(Figure 3), a relatively good monodispersity was obviousfor the γ‐[email protected]‐EG‐Cu(II) structure. Interestingly,it is evident that a dark γ‐Fe2O3 core with an average sizeof about 10–20 nm was surrounded by a grey titania shellwith a thickness of about 5–10 nm in the catalyststructure (Figure 3).
TGA/DTG study of γ‐[email protected]‐EG‐Cu(II) wasconducted to investigate the thermal stability of thecatalyst, as well as the amount of immobilized organicfunctional groups on the support (Figure 4). As can beseen in the TGA thermogram, the observed weight loss
FIGURE 5 EDS analysis of γ‐[email protected]‐EG‐Cu(II)
FIGURE 6 Magnetization curves of (a) γ‐[email protected]
nanoparticles and (b) γ‐[email protected]‐EG‐Cu(II)
6 of 12 NEJATIANFAR ET AL.
at temperatures below 200 °C was related to the adsorbedwater molecules on the support. Then, the decompositionof organic motifs occurred at temperatures ranging from200 to 670 °C (17.23 wt%). Based on the TGA results, theamount of organic backbone supported on γ‐[email protected]
is estimated to be 0.70 mmol g−1. These results were in agood agreement with the elemental analysis data(N = 3.01% and C = 7.02%) and ICP analysis. The ICPanalysis indicated that 0.74 mmol of copper was anchoredon 1.00 g of the catalyst.
EDS analysis disclosed the existence of C, O, Fe, Tiand Cu elements (Figure 5). This analysis well demon-strated that Cu(II) is immobilized on the guanidinatedepibromohydrin‐functionalized γ‐[email protected].
The magnetic properties of γ‐[email protected] and γ‐[email protected]‐EG‐Cu(II) were measured at ambienttemperature using VSM. As indicated in Figure 6, thesaturation magnetization values for γ‐[email protected] andγ‐[email protected]‐EG‐Cu(II) were 23.79 and 22.12 emu g−1,respectively. Indeed, the absence of hysteresis phenome-non indicated that both γ‐[email protected] and γ‐
[email protected]‐EG‐Cu(II) have superparamagnetism atroom temperature. A slight decrease in the saturationmagnetization of γ‐[email protected] after the surface graftingcould be attributed to the contribution of thenon‐magnetic materials.
3.2 | Catalytic synthesis of 2,4,5‐Trisubstituted and 1,2,4,5‐TetrasubstitutedImidazoles in presence of γ‐[email protected]‐
To evaluate and optimize the catalytic behaviour of γ‐[email protected]‐EG‐Cu(II) in the synthesis of imidazoles,initially a multicomponent condensation reaction for thepreparation of 2,4,5‐triphenyl‐1H‐imidazole was studiedunder various conditions (including different solvents,temperatures, amounts of catalyst and molar ratios ofreactants). The results are summarized in Table 1. As afirst step, to monitor whether the use of γ‐[email protected]‐
EG‐Cu(II) is crucial for this transformation, the multi-component condensation reaction of benzil (1 mmol),benzaldehyde (1 mmol) and ammonium acetate(2.5 mmol) at 100 °C was conducted under solvent‐freecondition in the absence of γ‐[email protected]‐EG‐Cu(II)and also in the presence of γ‐[email protected], γ‐[email protected]‐E and γ‐[email protected]‐EG (Table 1, entries1–4). The obtained results clearly indicate [email protected]‐EG‐Cu(II) is a vital catalyst for this conden-sation reaction (compare entry 5 with entries 1–4). It isinteresting to note that temperature plays an importantrole in the catalytic synthesis of 2,4,5‐triphenyl‐1H‐imid-azole. To get more insight into the temperature effect,the model reaction was performed in the temperaturerange 90–120 °C. At 90 °C the reaction was completedin a prolonged time, while further increasing the reactiontemperature (110 and 120 °C) had no great influence onthe reaction rate (Table 1, entries 6–8). Hence, 100 °Cwas selected as the optimum temperature to accomplish
TABLE 1 Optimization of various reaction parameters for one‐pot synthesis of 2,4,5‐triphenyl‐1H‐imidazole
EntryMolar ratio of benzaldehyde:benzil:ammonium acetate
1 1:1:2.5 — 100 — 60/24 (h) 0/0
2a 1:1:2.5 0.03 (g) 100 — 60 Trace
3b 1:1:2.5 0.03 (g) 100 — 60 Trace
4c 1:1:2.5 0.03 (g) 100 — 60 Trace
5 1:1:2.5 2.5 100 — 20 98
6 1:1:2.5 2.5 110 — 20 98
7 1:1:2.5 2.5 120 — 20 98
8 1:1:2.5 2.5 90 — 30 98
9 1:1:2.5 1.6 100 — 25 90
10 1:1:2.5 3.2 100 — 20 98
11 1:1:2.5 4 100 — 20 98
12 1:1:2 2.5 100 — 30 96
13 1:1:3 2.5 100 — 20 98
14 1:1:3.5 2.5 100 — 20 98
15 1:1:2.5 2.5 Reflux H2O 60 70
16 1:1:2.5 2.5 Reflux EtOH 60 78
17 1:1:2.5 2.5 Reflux CH3CN 60 73
aReaction performed in the presence of γ‐[email protected] performed in the presence of γ‐Fe2O[email protected]‐E.cReaction performed in the presence of γ‐[email protected]‐EG.
NEJATIANFAR ET AL. 7 of 12
the reaction. To further develop the progress of reaction interms of efficiency and time, the model reaction was car-ried out in the presence of various amounts of the catalyst.By applying lower catalytic amount (1.6 mol%), the prod-uct yield was found to be 90% in longer reaction time(Table 1, entry 9), whereas using higher amounts of cata-lyst (3.2 and 4 mol%) did not have any substantial effecton the reaction progress (Table 1, entries 10 and 11). Toexplore the effect of molar ratio of reactants on the reac-tion rate, we also implemented three separate experi-ments by applying 1:1:2, 1:1:3 and 1:1:3.5 molar ratios ofbenzaldehyde:benzil:ammonium acetate at 100 °C, undersolvent‐free condition (Table 1, entries 12–14). By using1:1:2 molar ratio, the reaction rate was not so satisfactory.However, additional amounts of ammonium acetate didnot have any noticeable influence on the reaction prog-ress. Accordingly, the optimal molar ratio of benzalde-hyde:benzil:ammonium acetate was selected as 1:1:2.5.To investigate the effect of solvent, the model reactionwas carried out in H2O, EtOH and CH3CN (Table 1,entries 15–17). It was found that conducting the reactionunder solvent‐free condition generates the desired prod-uct in excellent yield within a short reaction time, incomparison with the use of solvent (compare entry 5 withentries 15–17).
After optimizing the reaction conditions, to show thegeneral applicability of the present method, the reactionof benzil with a wide variety of aldehydes (aromatic,heteroaromatic and aliphatic) and ammonium acetatewas investigated under the optimized conditions(Table 2). A broad range of aromatic aldehydes bearingboth electron‐donating and electron‐withdrawing substit-uents underwent the successful one‐pot, multicomponentcyclocondensation reactions to provide 2,4,5‐trisubsti-tuted imidazoles in excellent yields (Table 2, entries 1–15). Interestingly, heteroaromatic aldehydes as well asaliphatic aldehydes also afforded the corresponding imid-azoles in high yields (Table 2, entries 16–19). In general,the aspect of this protocol is broad, since variousfunctional groups were found to be compatible undersuch reaction conditions.
To widen the applicability of the present protocol, syn-thesis of 1,2,4,5‐tetrasubstituted imidazoles was alsoinvestigated via the one‐pot, multicomponent condensa-tion reactions of benzil, aromatic aldehydes, ammoniumacetate and a selection of primary aromatic amines, underthe optimized conditions established for the preparationof 2,4,5‐trisubstituted imidazoles (Table 3). As can beseen, electron‐withdrawing substituents on aromatic ringof aldehyde and electron‐donating substituents on
TABLE 2 Synthesis of various 2,4,5‐trisubstituted imidazoles in presence of γ‐[email protected]‐EG‐Cu(II) under solvent‐free condition
Entry R Product Time (min) Isolated yield (%)
1 C6H5 3a 20 98
2 4‐NO2C6H4 3b 25 95
3 4‐CNC6H4 3c 25 95
4 4‐FC6H4 3d 25 90
5 4‐ClC6H4 3e 20 95
6 2‐ClC6H4 3f 30 95
7 3‐BrC6H4 3 g 30 95
8 4‐MeOC6H4 3 h 30 90
9 2‐MeOC6H4 3i 25 96
10 4‐MeC6H4 3j 20 95
11 2‐MeC6H4 3 k 20 98
12 4‐OHC6H4 3 l 30 90
13 2‐OHC6H4 3 m 25 92
14 4‐iprC6H4 3n 30 91
15 4‐(CH3)2NC6H4 3o 30 85
16 C4H4N 3p 37 92
17 2‐C4H3S 3q 20 90
18 C5H11 3r 25 95
19 C6H13 3 s 28 93
TABLE 3 Synthesis of various 1,2,4,5‐tetrasubstituted imidazoles in presence of γ‐[email protected]‐EG‐Cu(II) under solvent‐free condition
Entry R R′ Product Time (min) Isolated yield (%)
1 C6H5 C6H5 3 t 25 98
2 4‐ClC6H4 C6H5 3u 20 92
3 2‐CH3OC6H4 C6H5 3v 27 94
4 C6H5 4‐CH3C6H4 3w 18 90
5 C6H5 4‐CH3OC6H4 3x 15 90
6 C6H5 4‐ClC6H4 3y 28 90
7 C6H5 C6H5CH2 3z 23 92
8 of 12 NEJATIANFAR ET AL.
aromatic ring of primary amines could almost equallyaccelerate the corresponding condensation reactions.Generally, the reactions were clean and no side productswere detected. In all cases, the reactions proceeded
efficiently and gave the corresponding products in goodto excellent yields within short reaction times.
In our experiments, the completion of the reaction isconfirmed by the disappearance of aldehydes determined
NEJATIANFAR ET AL. 9 of 12
using TLC, followed by the appearance of a strong sharpabsorption band in the FT‐IR spectra of the products ataround 3338 or 1540 cm−1 and a medium absorption bandat 1666 cm−1, which are assigned to N─H or C─N andC═N stretching vibrations of 2,4,5‐trisubstituted imidaz-oles or 1,2,4,5‐tetrasubstituted imidazoles, respectively.All of the obtained products were known and their phys-ical data (colour, melting points) and spectral data (massspectrometry) were found to be identical with those ofauthentic compounds. Selected compounds were furtheridentified using FT‐IR, 1H NMR and 13C NMR spectros-copies, the results of which were compared with literaturedata. A diagnostic 1H NMR signal at around 12.70–11.20 ppm is assigned to the NH of 2,4,5‐trisubstitutedimidazoles. In 13C NMR spectra, a signal at around157.33–144.04 or 150.71–137.54 ppm is allocated to C‐2of 2,4,5‐trisubstituted imidazoles or 1,2,4,5‐tetrasubstituted imidazoles, respectively. See thesupporting information for details.
A postulated mechanism for this reaction is shown inScheme 3. The crucial catalytic role of γ‐[email protected]‐EG‐Cu(II) in this condensation reaction was established byperforming the reaction in the absence of γ‐[email protected]‐EG‐Cu(II). In this context, even after a longreaction time, no product was obtained (Table 1, entry 1).It is speculated that the nucleophilic attack of the ammo-nia nitrogen (obtained from NH4OAc) on the activatedcarbonyl group of aldehyde results in formation of aryl
SCHEME 3 Proposed mechanism for
formation of 2,4,5‐trisubstituted and
1,2,4,5‐tetrasubstituted imidazoles in the
presence of γ‐[email protected]‐EG‐Cu(II)
aldimine I. Subsequently, the catalyst facilitates the for-mation of intermediate II, by increasing the electrophilic-ity of the C═N on the aryl aldimine I towards thenucleophilic attack of ammonia or amine. There is no ten-dency between benzil and ammonia to produce α‐iminoketone I′. To understand which component (aldehyde orbenzil) is more reactive toward ammonia, in two separateflasks, NH4OAc was treated in turn with aldehyde andbenzil under optimized reaction conditions, using stoi-chiometric amounts of the reactants. The rapid reactionof aldehyde with NH4OAc produced aryl aldimine I,which next led to facile formation of intermediate II whentreated with NH4OAc or amine. On the other hand, atrace amount of α‐imino ketone I′ was produced fromthe reaction of benzil with NH4OAc or amine after aprolonged time. When the progress of the reaction mix-ture was followed precisely, α‐imino ketone I′ was notdetected. So, according to the above results, we candeduce that in the presence of aldehyde, nucleophilicattack of NH4OAc or amine on benzil is not successful.Intermediate II, in the presence of γ‐[email protected]‐EG‐Cu(II), condenses with benzil to form intermediate IIIor III′ which in turn rearranges to 2,4,5‐trisubstitutedimidazole or 1,2,4,5‐tetrasubstituted imidazole by a [1,5]hydrogen shift or dehydration, respectively, and then there‐generated catalyst re‐enters the catalytic cycle.
The recovery and reusability of the catalyst wereexamined in the synthesis of 2,4,5‐triphenyl‐1H‐
10 of 12 NEJATIANFAR ET AL.
imidazole. In this regard, after completion of the reaction,the reaction mixture was dissolved in hot ethanol and thecatalyst was separated using an external magnet. Then thecatalyst was washed with ethanol, air‐dried and stored forsubsequent reaction runs. The product was obtained in98, 98, 97, 95, 92 and 89% isolated yields in six consecutiveruns, which evidently indicated that the catalyst could bereused for at least six runs without loss of its activity(Figure 7).
TABLE 4 Comparison of catalytic activity of present catalyst with that
imidazole and 1,2,4,5‐tetraphenylimidazole
Entrya Catalyst (loading) Rea
1 ZrO2‐β‐CDb (40 mol%) Solv
2 Yb (OTf)3 (5 mol%) HO
3 Zinc(II) [tetra(4‐methylphenyl)] (2 μmol%) EtO
4 L‐Proline (15 mol%) MeO
5 Polymer–ZnCl2 (0.102 g) EtO
6 Alumc (0.3 g) EtO
7 InCl3.3H2O (10 mol%) MeO
8 Silica sulfuric acid (0.5 g) H2O
9 I2 (5 mol%) EtO
10 γ‐[email protected]‐EG‐Cu(II) (2.5 mol%) Solv
11 TiCl4.SiO2 (50 mol%) Solv
12 BF3.SiO2 (0.32 g) Solv
13 I2 (10 mol%) EtO
14 SBPPSAd (0.25 g) Solv
15 PEG‐400 (1.5 g) PEG
16 DABCO (0.7 mol%) t‐Bu
17 γ‐[email protected]‐EG‐Cu(II) (2.5 mol%) Solv
aEntries 1–10 refer to synthesis of 2,4,5‐triphenyl‐1H‐imidazole. Entries 11–16 refbZrO2‐supported‐β‐cyclodextrin.cPotassium aluminium sulfate.dSilica‐bonded propylpiperazine‐N‐sulfamic acid.
It is important to note that the FT‐IR spectrum of thenanocatalyst recovered after the sixth run (Figure 1e)indicated the entire preservation of the position, shapeand relative intensity of the indicative absorption bands.These data verified that no substantial changes happenedto the chemical structure of the functional groups andhydrogen bonding network of the nanocatalyst.
Also, it is noteworthy that the copper content of thefreshly prepared catalyst which was obtained using ICP
FIGURE 7 Synthesis of 2,4,5‐triphenyl‐
1H‐imidazole in the presence of reused γ‐[email protected]‐EG‐Cu(II). (*data refer to
conversion of benzaldehyde)
of some other reported methods in preparation of 2,4,5‐triphenyl‐1H‐
ction conditions Time (min) Yield (%)
ent‐free/100 °C 24 96
Ac/70 °C 120 95
H/ultrasound/r.t. 70 94
H/reflux 540 90
H/reflux 240 96
H/70 °C 150 93
H/r.t. 480 82
/reflux 240 73
H/75 °C 15 99
ent‐free/100 °C 15 98 (present study)
ent‐free /110 °C 190 75
ent‐free/140 °C 120 92
H/75 °C 50 96
ent‐free/140 °C 60 90
‐400/110 °C 360 86
OH/60 °C 720–900 92
ent‐free/100 °C 20 98 (present study)
er to synthesis of 1,2,4,5‐tetraphenylimidazole.
NEJATIANFAR ET AL. 11 of 12
analysis was 0.74 mmol of Cu per gram of the catalyst,while ICP analysis indicates that the catalyst after thesixth run comprises 0.68 mmol of Cu per gram. Fascinat-ingly, the amount of copper leached from the surface ofthe catalyst is very low.
To show the merits of the γ‐[email protected]‐EG‐Cu(II)nanocatalyst over some catalysts previously reported inthe literature, the catalytic performance of γ‐[email protected]‐EG‐Cu(II) in the preparation of 2,4,5‐triphenyl‐1H‐imidazole and 1,2,4,5‐tetraphenyl‐imidazolewas compared with that of various reported catalysts(Table 4). As can be observed, although all of theprotocols in Table 4 were able to produce good yields ofdesired products, some of them suffer from long reactiontimes to achieve such suitable yields (Table 4, entries 2–8, 11, 12 and 13–17) and the use of hazardous catalysts(Table 4, entries 9 and 13). However, the main drawbacksof almost all existing methods are difficult and tediouswork‐up procedures and most significantly none of themare magnetically recoverable. So, this comparison clearlyindicates that the present protocol is better in terms ofshorter reaction time and cleaner reaction media due toutilization of a green, nontoxic, nanomagnetic andeco‐benign recyclable catalyst.
4 | CONCLUSIONS
In this research we attempted to expand the application ofγ‐[email protected]‐EG‐Cu(II) as an effective and environ-mentally benign nanomagnetic catalyst in organicreactions. In this sense, a new and efficient procedurefor the preparation of 2,4,5‐trisubstituted and 1,2,4,5‐tetrasubstituted imidazoles under solvent‐free conditionis reported. Compared with traditional methods, thesignificant features of the current nanocatalyst in thereported approach are high yields of products, short reac-tion times, green reaction media, simple procedure, highatom economy and very wide range of substrates. More-over, the presented catalytic system is non‐volatile, non‐explosive, easy to handle, thermally robust and mustimportantly magnetically recyclable for at least six cycleswithout any appreciable loss in its catalytic activity.
The authors gratefully acknowledge the partial support ofthis study by Ferdowsi University of Mashhad ResearchCouncil (grant no. 3/43955).
Batool Akhlaghinia http://orcid.org/0000-0002-9940-5045
 J. G. Lambardino, E. H. Wiseman, J. Med. Chem. 1979, 17, 1182.
 T. N. Doman, S. L. McGovern, B. J. Witherbee, T. P. Kasten, R.Kurumbail, W. C. Stallings, D. T. Connolly, B. K. Shoichet,J. Med. Chem. 2002, 45, 2213.
 T. Maier, R. Schmierer, K. Bauer, H. Bieringer, H. Buerstell, B.Sachse, US Patent 4820335, 1989.
 M. E. Pierce, D. J. Carini, G. F. Huhn, G. J. Wells, J. F. Arnett,J. Org. Chem. 1993, 58, 4642.
 L. L. Chang, K. L. Sidler, M. A. Cascieri, S. Laszlo, G. Koch, B.Li, M. MacCoss, N. Mantlo, S. O'Keefe, M. Pang, A. Rolando, W.K. Hagmann, Bioorg. Med. Chem. Lett. 2001, 11, 2549.
 T. F. Gallagher, S. M. Fier‐Thompson, R. S. Garigipati, M. E.Sorenson, J. M. Smietana, D. Lee, P. E. Bender, J. C. Lee, J. T.Laydon, D. E. Griswold, M. C. Chabot‐Fletcher, J. J. Breton, J.L. Adams, Bioorg. Med. Chem. Lett. 1995, 5, 1171.
 P. Wasserscheid, W. Keim, Angew. Chem. Int. Ed. Engl. 2000,39, 3772.
 D. Bourissou, O. Guerret, F. P. Gabbai, G. Bertrand, Chem. Rev.2000, 100, 39.
 I. Satoru, Japn Kokkai Tokyo Koho JP 01, 117, 867, Chem.Abstr. 1989, 111, 214482.
 a) H. Debus, Eur. J. Org. Chem. 1858, 107, 199. b) B.Radziszewski, Eur. J. Inorg. Chem. 1882, 15, 1493.
 E. Kolvari, N. Koukabi, M. M. Hosseini, Z. Khandani, RSC Adv.2015, 5, 3682.
 S. Kantevari, S. V. N. Vuppalapati, O. B. Dhanraj, L. Nagarapu,J. Mol. Catal. A 2007, 266, 109.
 S. Balalaie, A. Arabanian, Green Chem. 2000, 2, 274.
 A. R. Karimi, Z. Alimohammadi, M. M. Amini, Molec. Divers.2010, 14, 635.
 S. Rostamnia, E. Doustkhah, Synlett 2015, 26, 1345.
 A. Teimouri, A. N. Chermahini, J. Mol. Catal. A 2011, 346, 39.
 N. Aziizi, Z. Manochehri, A. Nahayi, S. Torkashvand, J. Mol.Liq. 2014, 196, 153.
 Z. Zarnegar, J. Safari, New J. Chem. 2014, 38, 4555.
 S. D. Sharma, P. Hazarika, D. Konwar, Tetrahedron Lett. 2008,49, 2216.
 M. M. Heravi, K. Bakhtiari, H. A. Oskooie, S. Taheri, J. Mol.Catal. A 2007, 263, 279.
 L. Nagarapu, S. Apuri, S. Kantevari, J. Mol. Catal. A 2007,266, 104.
 A. R. Karimi, Z. Alimohammadi, J. Azizian, A. A. Mohammadi,M. R. Mohmmadizadeh, Catal. Commun. 2006, 7, 728.
 M. Kidwai, P. Mothsra, V. Bansal, R. K. Somvanshi, A. S.Ethayathulla, S. Dey, T. P. Singh, J. Mol. Catal. A 2007, 265, 177.
 M. M. Heravi, F. Derikvand, F. F. Bamoharram, J. Mol. Catal. A2007, 263, 112.
 A. Y. Usyatinsky, Y. L. Khemelnitsky, Tetrahedron Lett. 2000,41, 5031.
 F. H. Seyedeh, A. N. Seyede, B. Zahra, Monatsh. Chem. 2012,144, 387.
12 of 12 NEJATIANFAR ET AL.
 F. Xu, N. Wang, Y. Tian, G. Li, J. Heterocycl. Chem. 2013,50, 668.
 G. Sharma, Y. Jyothi, P. Lakshmi, Synth. Commun. 2006,36, 2991.
 S. Sarshar, D. Siev, M. M. Mjalli, Tetrahedron Lett. 1996, 37, 835.
 A. Shaabani, A. Rahmati, J. Mol. Catal. A 2006, 249, 246.
 J. N. Sngshetti, N. D. Kokare, S. A. Kotharkara, D. B. Shinde,J. Chem. Sci. 2008, 120, 463.
 D. Song, C. Liu, S. Zhang, G. Luo, Synth. React. Inorg. Met.‐Org.Chem. 2010, 40, 145.
 L. M. Wang, Y. H. Wang, H. Tian, Y. F. Yao, J. H. Shao, B. Liu,J. Fluorine Chem. 2006, 127, 1570.
 A. Maleki, R. Paydar, RSC Adv. 2015, 5, 33177.
 S. N. Murthy, B. Madhav, Y. V. D. Nageswar, Tetrahedron Lett.2010, 51, 5252.
 M. M. Heravi, F. Derikv, M. Haghighi, Monatsh. Chem. 2008,139, 31.
 C. Mukhopadhyay, P. K. Tapaswi, M. G. B. Drew, TetrahedronLett. 2010, 51, 3944.
 S. Samai, G. C. Nandi, P. Singh, M. S. Singh, Tetrahedron Lett.2009, 65, 10155.
 R. H. Shoar, G. Rahimzadeh, F. Derikvand, M. Farzaneh, Synth.Commun. 2010, 40, 1270.
 A. Hasaninejad, A. Zare, M. Shekouhy, J. Ameri Rad, J. Comb.Chem. 2010, 12, 844.
 a) R. Jahanshahi, B. Akhlaghinia, RSC Adv. 2016, 6, 29210. b)N. Razavi, B. Akhlaghinia, RSC Adv. 2015, 5, 12372. c) S. S. E.Ghodsinia, B. Akhlaghinia, RSC Adv. 2015, 5, 49849. d) R.Jahanshahi, B. Akhlaghinia, RSC Adv. 2015, 5, 104087. e) M.Zarghani, B. Akhlaghinia, Appl. Organometal. Chem. 2015, 29,683. f) M. Zarghani, B. Akhlaghinia, RSC Adv. 2015, 5, 87769.g) Z. Zareie, B. Akhlaghinia, Chem. Pap. 2015, 69, 1421. h) M.Zarghani, B. Akhlaghinia, RSC Adv. 2016, 6, 31850. i) N. Razavi,B. Akhlaghinia, New J. Chem. 2016, 40, 447. j) N. YousefiSiavashi, B. Akhlaghinia, M. Zarghani, Res. Chem. Intermed.2016, 42, 5789. k) S. S. E. Ghodsinia, B. Akhlaghinia, R.Jahanshahi, RSC Adv. 2016, 6, 63613. l) Z. Zarei, B.Akhlaghinia, RSC Adv. 2016, 6, 106473. m) M. Zarghani, B.Akhlaghinia, Bull. Chem. Soc. Jpn. 2016, 89, 1192. n) R.Jahanshahi, B. Akhlaghinia, Chem. Pap. 2017, 71, 1351. o) N.Razavi, B. Akhlaghinia, R. Jahanshahi, Catal. Lett. 2017, 147,360. p) M. Esmaielpour, B. Akhlaghinia, R. Jahanshahi,J. Chem. Sci. 2017, 129, 313. q) S. M. Masjed, B. Akhlaghinia,M. Zarghani, N. Razavi, Aust. J. Chem. 2017, 70, 33. r) E.Karimian, B. Akhlaghinia, S. S. E. Ghodsinia, J. Chem. Sci.
2016, 128, 429. s) R. Jahanshahi, B. Akhlaghinia, New J. Chem.2017, 41, 7203.
 S. Sobhani, Z. Vahidi, Z. Zeraatkar, S. Khodadadi, RSC Adv.2015, 5, 36552.
 A. Banisharif, S. H. Elahi, A. F. Anaraki, A. A. Khodadadi, Y.Mortazavi, IJNN 2013, 9, 193.
 a) Y. Gao, Y. Masuda, Z. Peng, T. Yonezawa, K. Koumoto,J. Mater. Chem. 2003, 13, 608. b) B. Klingenberg, M. A. Vannice,Chem. Mater. 1996, 8, 2755. c) A. Rostami, B. Atashkar, D.Moradi, Appl. Catal. A 2013, 467, 7.
 F. Adam, K. M. Hello, H. Osman, Chin. J. Chem. 2010, 28, 2383.
 Y. R. Girish, K. S. S. Kumar, K. N. Thimmaiah, K. S. Rangappa,S. Shashikanth, RSC Adv. 2015, 5, 75533.
 J. Safari, S. D. Khalili, S. H. Banitaba, H. Dehghani, J. KoreanChem. Soc. 2011, 55, 1.
 L. Wang, C. Cai, Monatsh. Chem. 2009, 140, 541.
 A. A. Mohammadi, M. Mivechi, H. Kefayati, Monatsh. Chem.2008, 139, 935.
 B. F. Mirjalili, A. H. Bamoniri, L. Zamani, Sci. Iran. 2012,19, 565.
 B. Sadeghi, B. B. F. Mirjalili, M. M. Hashemi, Tetrahedron Lett.2008, 49, 2575.
 M. Kidwai, P. Mothsra, Tetrahedron Lett. 2006, 47, 5029.
 K. Niknam, A. Deris, F. Naeimi, F. Majleci, Tetrahedron Lett.2011, 52, 4642.
 X. C. Wang, H. P. Gong, Z. J. Quan, L. Li, H. L. Ye, Chin. Chem.Lett. 2009, 20, 44.
Additional Supporting Information may be found onlinein the supporting information tab for this article.
How to cite this article: Nejatianfar M,Akhlaghinia B, Jahanshahi R. Cu(II) immobilizedon guanidinated epibromohydrin‐functionalized γ‐[email protected] (γ‐[email protected]‐EG‐Cu(II)): A highlyefficient magnetically separable heterogeneousnanocatalyst for one‐pot synthesis of highlysubstituted imidazoles. Appl Organometal Chem.2017;e4095. https://doi.org/10.1002/aoc.4095